Electrospun conducting polymer nanofibers and electrical ......
Embed Size (px)
Transcript of Electrospun conducting polymer nanofibers and electrical ......
Journal of Bioscience and Bioengineering VOL. 112 No. 5, 501–507, 2011
Electrospun conducting polymer nanofibers and electrical stimulation of nerve stem cells
Molamma P. Prabhakaran,1,⁎ Laleh Ghasemi-Mobarakeh,2 Guorui Jin,3 and Seeram Ramakrishna3
⁎ Correspond E-mail add
Nanoscience and Nanotechnology Initiative, Health Care and Energy Materials Laboratory, Faculty of Engineering, 2 Engineering Drive 3, National University of Singapore, Singapore 117576,1 Islamic Azad University, Najafabad branch, Isfahan, Iran,2 and Department of Mechanical
Engineering, National University of Singapore, 2 Engineering Drive 3, Singapore 1175763
Received 11 January 2011; accepted 9 July 2011 Available online 2 August 2011
Tissue engineering of nerve grafts requires synergistic combination of scaffolds and techniques to promote and direct neurite outgrowth across the lesion for effective nerve regeneration. In this study, we fabricated a composite polymeric scaffold which is conductive in nature by electrospinning and further performed electrical stimulation of nerve stem cells seeded on the electrospun nanofibers. Poly-L-lactide (PLLA) was blended with polyaniline (PANi) at a ratio of 85:15 and electrospun to obtain PLLA/PANi nanofibers with fiber diameters of 195±30 nm. The morphology, chemical and mechanical properties of the electrospun PLLA and PLLA/PANi scaffolds were carried out by scanning electron microscopy (SEM), X-ray photo electron spectroscopy (XPS) and tensile instrument. The electrospun PLLA/PANi fibers showed a conductance of 3×10−9 S by two-point probe measurement. In vitro electrical stimulation of the nerve stem cells cultured on PLLA/PANi scaffolds applied with an electric field of 100 mV/mm for a period of 60 min resulted in extended neurite outgrowth compared to the cells grown on non-stimulated scaffolds. Our studies further strengthen the implication of electrical stimulation of nerve stem cells on conducting polymeric scaffolds towards neurite elongation that could be effective for nerve tissue regeneration.
© 2011, The Society for Biotechnology, Japan. All rights reserved.
[Key words: Polyaniline; Conducting polymer; Poly-L-lactide; Neurite elongation; Nerve tissue engineering]
A successful tissue engineered product is such that the scaffold should have the ability to control the cellular response to direct the particular repair and regeneration of the concerned tissue. Nerve regeneration after injury is highly influenced by the cellular environment and several factors including the scaffold topography, stimulations (electrical, mechanical) or engineered channels affect the neurite outgrowth and axonal elongation (1,2). Directional cues can be provided using patterned nano extracellular matrix (ECM) structures, but theymay notmaintain the therapeutic levels of growth promoting signals which limits the nerve regeneration process in vivo (3). Growth factors such as the nerve growth factor (NGF) and brain derived neurotrophic factor (BDNF) have been delivered to the site of injury to promote axonal growth or methods such as the modification of biomaterial surfaces using peptides or proteins are being carried out. However, such methods involve limitations of retaining the bioactivity of the molecules and providing controlled and localized delivery to the site of injury (4–7). Electrical stimulation is an effective cue for stimulating cell proliferation and differentiations, mainly because bioelectricity plays an integral role in maintaining biological functions such as signaling of the nervous system. Moreover, recent studies on the electrical stimulation of cells cultured on conducting
ing author. Tel.: +65 6516 4272; fax: +65 6773 0339. ress: [email protected] (M.P. Prabhakaran).
- see front matter © 2011, The Society for Biotechnology, Japan. All .jbiosc.2011.07.010
polymeric substrates have shown positive cellular influence in supporting and modulating certain kinds of tissue regeneration including the nerve (8,9).
Synthetic polymers have been widely studied for neural implanta- tions, and bio-resorbable materials hold great flexibility in mechanical and chemical properties, lack antigenicity and avoid problems associ- ated of chronic persistence (10). Polyglycolide (PGA), polylactide (PLA) and PLGA have been employed for use as nerve grafts, but the potential problem associated with PLGA is its fast degradation properties resulting in the collapse and inhibition of axonal growth (11). Poly(L-lactic acid) (PLLA) possesses good mechanical integrity, biodegradability and biocompatibility and it is utilized for the fabrication of scaffolds for nerve regeneration (11). PLLA has shown longer degradation behaviors and researchers have also used PLLA microfilaments as structural support for long lesion nerve gap regeneration (12). On the other hand, polyaniline (PANi) has attracted special attention because of its ease of synthesis, low cost, conductivity and environmental stability (13,14). Composite scaffolds of PANi with gelatin were fabricated by Li et al. (14) recently, where they found the fibers supporting the proliferation of H9c2 rat cardiac myoblasts (14). However, there are very limited studies carried out on the cellular response of bioengineered electroactive substrates for nerve tissue engineering. In this study, we investigated the effect of incorporation of PANi to PLLA towards the electro-spinnability of PLLA/PANi nanofibers,
http://dx.doi.org/10.1016/j.jbiosc.2011.07.010 http://dx.doi.org/10.1016/j.jbiosc.2011.07.010 http://dx.doi.org/10.1016/j.jbiosc.2011.07.010 http://dx.doi.org/10.1016/j.jbiosc.2011.07.010 mailto:[email protected] http://dx.doi.org/10.1016/j.jbiosc.2011.07.010
502 PRABHAKARAN ET AL. J. BIOSCI. BIOENG.,
evaluated the morphology, surface characteristics, mechanical strength and conductance of the electrospun nanofibers. Electrical stimulations of nerve stem cells cultured on conducting polymeric scaffolds were further carried out to enhance the neurite outgrowth, thus strengthen- ing the application of electrical stimulus as a potential clue for nerve tissue regeneration, evenwithout thepresenceof differentiation growth factors.
MATERIALS AND METHODS
Materials PLLA with a molecular weight of 100,000 Da, was purchased from Polysciences (Warrington, PA, USA). 1,1,1,3,3,3-hexafluoro-2-propanol (HFP), poly- aniniline emeraldine base (PANi-EB) of MW 65,000, camphorsulfonic acid (CSA) and hexamethyldisilazane (HMDS) were purchased from Sigma-Aldrich (St. Louis, MO, USA). Dulbecco's modified Eagle's medium (DMEM), fetal bovine serum (FBS), horse serum (HS), antibiotics, and trypsin–ethylenediaminetetraacetic acid (EDTA) were purchased from Gibco (Invitrogen, Carlsbad, CA, USA). CellTiter 96 AQueous one solution was purchased from Promega, Madison, WI, USA.
Electrospinning of nanofibrous scaffolds PLLA was dissolved in HFP to obtain a 16% (w/v) solution and electrospun at a voltage of 10 kV (high voltage system, Gamma High Voltage Research, FL, USA), while the collector was placed at a distance of 15 cm from the needle tip to collect the nanofibers. Equal amounts of CSA and polyaniline-emeraldine base (PANi-EB) were dissolved in HFP, allowing the proton- ation of PANi-EB to a polyelectrolyte form. PANi-EB gets doped to polyaniline- emeraldine salt (PANi-ES) form, whereby the polymer undergoes an insulator to metal transition with change in conformation of the polymer backbone accommodating this electronic transformation (15). To the doped PANi solution, PLLA was added making a total concentration of 16% (w/v) and stirring was continued overnight. Before electrospinning, the polymer solution was filtered through a 0.22 μm filter unit and fed to a 5 ml standard syringe attached to 27 G blunted stainless steel needle using a syringe pump (KDS 100, KD Scientific, Holliston, MA, USA) at a flow rate of 1 ml/h. Electrospinning was carried out at a high voltage of 15 kV to obtain PLLA/PANi nanofibers. All experiments were performed in a humidity of less than 60% and a temperature of 22–24°C. Nanofibers were collected on 15 mm glass cover slips for cell culture experiments.
Characterization of nanofibrous scaffolds The morphology of electrospun nanofibers was studied using a scanning electron microscope (SEM) (JSM-5800LV, JEOL, Tokyo Japan) at an accelerating voltage of 10 kV, after sputter coating with gold (JEOL JFC-1200 Auto Fine Coater). The diameter of the electrospun nanofibers were also measured from the SEM micrographs using image analysis software (ImageJ, National Institutes of Health, Bethesda, MD, USA).
The wettability of the electrospun scaffolds was evaluated by water contact angle measurement using a VCA Optima Surface Analysis system (AST products, Billerica, MA). The droplet size was set at 0.5 μl. Average value of the contact angle was reported with standard deviation, after testing for a minimum of seven samples.
Attenuated total reflectance–Fourier transform infrared (ATR–FTIR) spectroscopic analysis of the electrospun nanofibrous scaffolds was performed on Avatar 380 spectrophotometer (Thermo Nicolet, Waltham, MA, USA) over a range of 400– 4000 cm−1 at a resolution of 2 cm−1with 64 scans per sample. The X-ray photoelectron spectroscopy (XPS) of PLLA and PLLA/PANi scaffolds were obtained from VG-Escalab 2201-XL Base system (Thermo VG Scientific, UK) at a take-off angle of 90°.
Tensile properties of the electrospun nanofibrous scaffolds were determined using a tabletop tensile tester (Instron 3345, Instron, Norwood, MA, USA) with a load cell capacity of 10 N. Rectangular specimens of dimensions 10 mm×20 mm were used for testing at a